salt=occluded zeolite waste forms: crystal /67531/metadc691562/m2/1/high_res_d/ salt=occluded
Post on 20-Mar-2020
Embed Size (px)
SALT=OCCLUDED ZEOLITE WASTE FORMS: CRYSTAL STRUCTURES AND TRANSFORMABILITY
J. W. RICHARDSON, JR. Intense Pulsed Neutron Source Division, Argonne National Laboratory, Argonne, L 60439 USA
The submitted manuscript has been authored by a contractor of the U. S. Government under contract W-3 1-109-ENG-38. Accordingly, the U. S. Government retains a nonexclusive, royalty-free license to publish or reproduce the published form of this contribution, or allow others to do so, for U. S. Government purposes.
Describing work presented at the Materials Research Society Meeting
Dec. 2-6, 1996 Boston, MS
Proceedings to be published in Mat. Res. SOC. Symp. Proc.
*Work supported by U. S . Department of Energy, BES, contract No. W-31-109-ENG-38
The submitted manuscript has be%n authored by a contractor of the U. S. Government under contract No, W-31-104ENG-38. Accordingly, the U. S. Government retains a nonexclusive, royalty-frea license to Publish or reproduce the plblirhed form of this contribution, or allow others to do 10. for
~ U. S. Govsrnment purpoosr. I
This report was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor any agency thereof, nor any of their employees, make any warranty, express or implied, or assumes any legal liabili- ty or responsibility for the accuracy, completeness, or usefulness of any information, appa- ratus, product, or process disdased, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, pmess, or service by trade name, trademark, manufacturer, or otherwise does not necessarily CorntitUte or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessar- ily state or reflect those of the United States Government or any agency thereof.
SALT-OCCLUDED ZEOLITE WASTE FORMS: CRYSTAL STRUCTURES AND TRANSFORMABILITY
Neutron diffraction studies of salt-occluded zeolite and zeolite/glass composite samples, sim- ulating nuclear waste forms loaded with fission products, have revealed complex structures, with cations assuming the dual roles of charge compensation and occlusion (cluster formation). These clusters roughly fill the 6-8 A diameter pores of the zeolites. Samples are prepared by equilibrat- ing zeolite-A with complex molten Li, K, Cs, Sr, Ba, Y chloride salts, with compositions repre- sentative of anticipated waste systems. Samples prepared using zeolite 4A (which contains exclu- sively sodium cations) as starting material are observed to transform to sodalite, a denser alumi- nosilicate framework structure, while those prepared using zeolite 5A (sodium and calcium ions) more readily retain the zeolite-A structure. Because the sodalite framework pores are much smaller than those of zeolite-A, clusters are smaller and more rigorously confined, with a corre- spondingly lower capacity for waste containment. Details of the sodalite structures resulting from transformation of zeolite-A depend upon the precise composition of the original mixture. The en- hanced resistance of salt-occluded zeolites prepared from zeolite 5A to sodalite transformation is thought to be related to differences in the complex chloride clusters present in these zeolite mix- tures. Data relating processing conditions to resulting zeolite composition and structure can be used in the selection of processing parameters which lead to optimal waste forms.
This work is carried out in support of a ceramic waste form development project at Argonne National Laboratory for salt waste generated from electrometallurgically conditioned spent nuclear fuel. The ceramic waste form IS prepared from hot isistatic pressing of a mixture of salt- occluded zeolite and glass binder. These composite materials were shown to be leach resistant (meeting standard criteria required for waste storage applications). While leach tests are generally satisfactory, however, some variability in performace has been observed.
Powder diffraction analysis of prospective zeolite waste form composites is important foi- correlating structural features with waste form capacity-controlling factors such as cation segre- gation, competition between charge balance and occlusion, mixed phase compositions and resis- tance to phase transformation during processing. This work has emphasized neutron diffraction for a number of reasons. Rietveld profile refinement of zeolite and molecular sieve structures us- ing neutron powder diffraction data is well established [ 1-41. In addition, the scattering contrast of important constituent elements in the composites is advantageous. These zeolite composites tend to exhibit strong long-range cation ordering. The strength of this ordering is evidenced by dramatic re-arrangement of oxygens in the zeolite framework to accommodate the long-range or- dering. Oxygen is a relatively weak scatterer of X-rays, but an exceptionally strong scatterer of neutrons. Neutron diffraction patterns which are strongly influenced by oxygen scattering, there- fore, allow us to follow in detail the accommodation of oxygen to waste salt occlusion. Furthermore, the scattering strength of Li is considerable with neutron diffraction, allowing us to recognize the strong impact Li has on the resulting structures.
Zeolites are very complex materials, even in their simplest chemical forms. Occlusion of simulated waste salts further complicates the structures, by producing strong distortions in A104 and Si04 tetrahedra in the zeolite. General statements can, however, be made regarding the rela- tionship between overall composition and resulting structure. This is because cations from the salt (Li in particular) dominate interactions with the zeolite, to induce surprisingly regular long- range structures. Salt-occluded zeolites with relatively high mass fractions of Li (2 4 wt%) crys- tallize in a single phase structure with nearly absolute long-range ordering of cations, largely on the basis of size [ 5 ] . As will be discussed in this paper, mixtures prepared from zeolite 4A (with exclusively Na+ cations) and from zeolite 5A (roughly 60% Ca2+, 40% Na+) also have structures
involving strong interactions between occluded salt complexes and the zeolite framework, but with different cation ordering schemes.
As part of the waste form processing, salt-occluded zeolites are pressure-bonded with borosilicate glass at an elevated temperature to form the final product. Under many circum- stances, this hgh-temperature processing results in transformation of zeolite-A to the more dense zeolite known as sodalite. The susceptibility of the occluded zeolite to this conversion depends on the starting material; samples prepared with zeolite 5A are less likely to convert. The structures of zeolite 4A and zeolite 5A mixtures have been determined in an effort to identify correlations between cation distribution, etc. and susceptibility to transformation.
Salt-occluded zeolite samples are prepared using one of three methods [6-81: (1) ion ex- change, (2) occlusion or (3) a combination of (1) and (2). In method (l), the zeolite is treated with an excess of salt, usually a factor of 10: 1 salt:zeolite, and ion exchange predominates. The concentration of fission products in the salt-occluded zeolite is high, usually over 10 wt% and there is little Na, c 1 wt%. Most charge compensating ions are Li and K. This type of salt-oc- cluded zeolite is referred to as fully exchanged zeolite. In method (2), excess zeolite is treated with a minimum of salt, and salt occlusion predominates. Typically, there is about 4 times as much zeolite as salt. Thus, the concentration of fission products in the salt-occluded zeolite is about 20% of that in the salt, about 1-3 wt%. The Na concentration is high, typically around 12- 13 wt%. This type of salt-occluded zeolite is referred to as blended zeolite. In method (3), both the ion exchange and the occlusion methods are combined. The zeolite is first treated with excess salt, as in an ion exchange process. The zeolite is fully exchanged but contains a significant amount of surface salt. This surface salt is sorbed into new zeolite using the occlusion or second method. The combination method leads to intermediate fission product and Na concentrations.
Shown in Table 1 are the chemical compositions of salt-occluded zeolites used in our neutron powder diffraction studies. These were chosen to be representative of each of the methods de- scribed above. Samples identified as BE-4 and BE-5 were prepared using method (1), 3023-E, 4A-Sr, 4A-Y, SA-Sr and 5A-Y were prepared using method (2), and 12223-D was prepared us- ing method (3).
Table 1. Chemical compositions (wt%) for some of the salt-occluded zeolites studied Ion Li+ Y h Na+ Ca2+ !# Baa K+ cs+ a-
B E 3 BE-5 4.00 4.00 0.46 1 .W 0.60 0.60
3.45 1.71 2.56 3.49 6.00 6.00 7.75 8.02 16.00 16.00
12223-D 1.29 0.0 1 7.04
0.06 0.19 14.60 0.67 12.60
3023-E 4A-Sr 4A-Y 1.72 1.14 1.30 0.00 1.52 11.20 12.80 13.00
0.6 1 0.48 5.15 4.45 5.00 1.38
12.60 11.30 12.00
SA-Sr SA-Y 1.25 1.22
3.01 3.49 3.83 7.66 7.45 3.24
Salt-occluded zeolite samples, prepared as loose powders, were transferred to vanadium sam- ple tubes and placed in the General Purpose Powder Diffractometer (GPPD)  at the Intense Pulsed Neutron Source (IPNS) at Argonn